Thermal, dielectrical and mechanical response of α and β-poly(vinilydene fluoride)/Co-MgO nanocomposites
© Paleo et al; licensee Springer. 2011
Received: 29 October 2010
Accepted: 25 March 2011
Published: 25 March 2011
Nanocomposites of the self-forming core-shell Co-MgO nanoparticles, which were of approximately 100 nm in diameter, and poly(vinylidene fluoride) (PVDF) polymer have been prepared. When the polymer is crystallized in the α-phase, the introduction of the nanoparticles leads to nucleation of the γ-phase of PVDF, increasing also the melting temperature of the polymer. With the introduction of the Co-MgO particles, the dielectric constant of the material slightly increases and the storage modulus decreases with respect to the values obtained for the pure polymer.
Nanosized metal and semiconductor particles possess unique electronic, optical, and catalytic properties that are different from those of bulk crystals. These properties make them attractive materials for fabricating hybrid composites based on a polymer matrix with nanoparticle fillers , allowing tailor-made electrical and optical composite responses. Among nanoscale fillers, Co and MgO structured particles are particularly promising candidates as they possess a variety of outstanding physicochemical properties which are utilized in the Fischer-Tropsch catalysis, the carbon nanotube synthesis, and for hydrogen storage applications. In addition, the combination of a magnetic-core and dielectric-shell to form a magnetic material with high permeability at high frequency may play an important role in satisfying the requirements for miniaturization of communication equipments [2, 3].
Poly(vinylidene fluoride) (PVDF) is the main representative of a family of polymeric materials with interesting scientific and technological properties. For instance, this polymer is known for its outstanding electroactive properties and an unusual high dielectric constant with respect to other polymers . Although the several studies exploring the properties of the polymer nanocomposites as a function of nanosized fillers in PVDF , only few studies are focused in systems with core-shell structures embedded in PVDF. For instance, Dang et al.  prepared Ag-TiO2/PVDF composites for studying the effect of core-shell structure on global dielectric permittivity in the nanocomposites. Petrychuk et al.  prepared Fe3O4 nanoparticles with and without shell of polyaniline dispersed in PVDF, focusing in dispersion and consequently influence in coefficient of squareness of the hysteresis loop and electromagnetic energy absorption.
In this study, nanocomposite films of PVDF in its α and β phases with core-shell Co-MgO nanoparticles were prepared by solution casting technique for different filler concentrations. The influence of the nanoparticles on the polymer phase, degree of crystallinity, mechanical behavior, and dielectric response of the composites was investigated.
Starting powders from Co (Aldrich, 99.8%, Madrid, Spain) and MgO (Alfa Aesar, 99.998%, Ward Hill, USA) were used for producing magnetic Co particles covered with MgO in a single-step process by means of vapor phase condensation . Nanocomposite samples of PVDF (Solef 1010 from Solvay) with magnetic Co-MgO particles were prepared by dispersing the nanoparticles in a solution of PVDF in N,N-dimethylformamide (DMF, pure grade from Merck, Darmstadt, Germany ). The initial concentration was 1 g of PVDF per mL of DMF. For obtaining a good dispersion, the magnetic nanoparticles within the solution were placed in an ultrasound bath for 8 h. Flexible films were obtained by spreading the solution on a clean glass substrate. Solvent evaporation and polymer crystallization were obtained inside an oven at controlled temperature. The samples in the α-phase were obtained by maintaining the inside an oven for 60 min at 120°C to ensure complete crystallization of the nanocomposite and solvent removal. After the crystallization process, samples were melted at 230°C for 15 min and cooled down at room temperature. Samples in the β-phase were obtained by solvent evaporation at room temperature. The volume fraction of the magnetic Co-MgO nanoparticles was varied from 0.02 to 0.20%.
The characterization of the crystalline phases present in each PVDF sample was achieved by Fourier transform infrared (FTIR) spectroscopy (Perkin-Elmer, model 1610) in attenuated total reflection mode at room temperature. The thermal stability of the nanocomposites was evaluated by means of differential scanning calorimetry (DSC) (Perkin-Elmer Pyris 1) at a heating rate of 10°C/min. Dynamical mechanical analysis (DMA) was carried out at room temperature (Perkin-Elmer DMA-8000), under nitrogen atmosphere. Finally, circular Au electrodes of 5 mm radius were vacuum evaporated onto both sides of each sample to evaluate the dielectric response of the nanocomposites. The real (ε") part of the permittivity and the dielectric losses (tan δ) were obtained in the frequency range 100 Hz to 1 MHz at room temperature with an automatic Quadtech 1929 Precision LCR meter.
Results and discussion
A detailed structural, morphological, and magnetic characterization of the samples has previously been published . Particles of about 100 nm diameter were chosen for this study. The magnesia coating not only protects the high magnetic moment (170 ± 8 emu/g) Co-fcc core from corrosion, but also brings about further improvement by providing polar surfaces for attachment of polymers.
The presence of the different phases and their nature was further confirmed by DSC. Thermograms for samples crystallized from the melt are shown in Figure 2b. The samples containing nanoparticles show two melting peaks. The first one is related to the melting of the α-phase of the polymer, the second one occurring at higher temperatures relates to the melting of the γ-PVDF. It is also observed that the incorporation of the Co-MgO nanoparticles into the polymeric matrix increases its thermal stability, as surmised from the slightly higher melting temperature of the nanocomposite. In this way, a method to obtain γ-PVDF at high or moderate cooling rates from the melt is obtained, without the need to apply thermal annealing at temperatures above 160°C for long term, the usual way to obtain this phase .
For samples crystallized at room temperature (data not shown), the dielectric response of the polymer is quite similar, and shows that the nanoparticles do not improve the dielectric response of the β-PVDF. With respect to the dynamical mechanical response, on the other hand, the pure α-phase matrix has highest mechanical properties when compared with the nanocomposite samples (Figure 3b), which can be related to defect formation around the nanoparticles, due to the interaction with the nanoparticle shell, and a decrease in the degree of crystallinity as observed in the DSC scans.
The introduction of Co-MgO core-shell fillers within a PVDF matrix influences the polymer crystallization. A stable MgO oxide shell protected the magnetic metallic Co core from oxidation to realize a high saturation magnetization, while altering the PVDF molecules packaging via Mg-OH bonding at the polymer/particle interface. The dielectric properties are slightly affected but, on the other hand, the storage modulus is strongly reduced.
Fourier transform infrared
The authors acknowledge the Foundation for Science and Technology, for the PTDC/CTM/69316/2006 grant, the NANO/NMed-SD/0156/2007 project, EU-DG RTD's SFERA (BIONANOS) and the Spanish MICINN (MAT2009-08024 and CSD2007-00041) for financial support. C. M. Boubeta gratefully acknowledges the financial support from the Spanish "Ramón y Cajal" program.
- Lewis LN: Chemical Catalysis By Colloids And Clusters. Chem Rev 1993, 93: 2693–2730. 10.1021/cr00024a006View ArticleGoogle Scholar
- Han Z, Li D, Wang H, Liu XG, Li J, Geng DY, Zhang ZD: Broad-band electromagnetic-wave absorption by FeCo/C nanocapsules (vol 95, 023114, 2009). Appl Phys Lett 2009, 95: 1.Google Scholar
- Liu XG, Li B, Geng DY, Cui WB, Yang F, Xie ZG, Kang DJ, Zhang ZD: (Fe, Ni)/C nanocapsules for electromagnetic-wave-absorber in the whole Ku-band. Carbon 2009, 47: 470–474. 10.1016/j.carbon.2008.10.028View ArticleGoogle Scholar
- Lovinger AJ: Developments in Crystalline Polymers. London: Applied Science Publications; 1981.Google Scholar
- Miranda D, Sencadas V, Sánchez-Iglesias A, Pastoriza-Santos I, Liz-Marzán LM, Gomez Ribelles JL, Lanceros-Mendez S: Influence of silver nanoparticles concentration on the alpha- to beta-phase transformation and the physical properties of silver nanoparticles doped poly(vinylidene fluoride) nanocomposites. J Nanosci Nanotechnol 2009, 9: 2910–2916. 10.1166/jnn.2009.208View ArticleGoogle Scholar
- Dang ZM, You SS, Zha JW, Song HT, Li ST: Effect of shell-layer thickness on dielectric properties in Ag@TiO2 core@shell nanoparticles filled ferroelectric poly(vinylidene fluoride) composites. Phys Status Solidi A Appl Mater 2009, 207: 739–742. 10.1002/pssa.200925471View ArticleGoogle Scholar
- Petrychuk M, Kovalenko V, Pud A, Ogurtsov N, Gubin A: Ternary magnetic nanocomposites based on core-shell Fe3O4/polyaniline nanoparticles distributed in PVDF matrix. Phys Status Solidi A Appl Mater 2010, 207: 442–447. 10.1002/pssa.200824421View ArticleGoogle Scholar
- Martinez-Boubeta C, Balcells L, Monty C, Martinez B: The effects of exchange bias on Fe-Co/MgO magnetic nanoparticles with core/shell morphology. J Phys Condens Matter 2010, 22: 5. 10.1088/0953-8984/22/2/026004View ArticleGoogle Scholar
- Silva MP, Sencadas V, Botelho G, Machado AV, Rolo AG, Rocha JG, Lanceros-Mendez S: [alpha]- and [gamma]-PVDF: crystallization kinetics, microstructural variations and thermal behaviour. Mater Chem Phys 2010, 122: 87–92. 10.1016/j.matchemphys.2010.02.067View ArticleGoogle Scholar
- Sencadas V, Gregorio R, Lanceros-Méndez S: α to β phase transformation and microestructural changes of PVDF films induced by uniaxial stretch. J Macromol Sci B Phys 2009, 48: 514–525. 10.1080/00222340902837527View ArticleGoogle Scholar
- He XJ, Yao K: Crystallization mechanism and piezoelectric properties of solution-derived ferroelectric poly(vinylidene fluoride) thin films. Appl Phys Lett 2006, 89: 3.Google Scholar
- Serantes D, Baldomir D, Martinez-Boubeta C, Simeonidis K, Angelakeris M, Natividad E, Castro M, Mediano A, Chen DX, Sanchez A, Balcells Ll, Martinez B: Influence of dipolar interactions on hyperthermia properties of ferromagnetic particles. J Appl Phys 2010, 108: 073918. 10.1063/1.3488881View ArticleGoogle Scholar
This article is published under license to BioMed Central Ltd. This is an Open Access article distributed under the terms of the Creative Commons Attribution License (http://creativecommons.org/licenses/by/2.0), which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.